Embed Size (px)
Structural, vibrational, and electronic topological transitions of Bi1.5Sb0.5Te1.8Se1.2under pressureJoon-Seok Kim, Rinkle Juneja, Nilesh P. Salke, Witold Palosz, Venkataraman Swaminathan, Sudhir Trivedi,Abhishek K. Singh, Deji Akinwande, and Jung-Fu Lin
Citation: Journal of Applied Physics 123, 115903 (2018); doi: 10.1063/1.5018857View online: https://doi.org/10.1063/1.5018857View Table of Contents: http://aip.scitation.org/toc/jap/123/11Published by the American Institute of Physics
Articles you may be interested inPressure-induced topological phase transitions and structural transition in 1T-TiTe2 single crystalApplied Physics Letters 112, 041907 (2018); 10.1063/1.5012842
Structure determination of the high-pressure phases of topological insulator Bi2Se3 using experiments andcalculationsJournal of Applied Physics 121, 225902 (2017); 10.1063/1.4985546
Strain-induced Dirac state shift in topological insulator Bi2Se3 nanowiresApplied Physics Letters 111, 171601 (2017); 10.1063/1.5001929
Doping induced enhanced density of states in bismuth tellurideApplied Physics Letters 111, 232101 (2017); 10.1063/1.4989602
Similar ultrafast dynamics of several dissimilar Dirac and Weyl semimetalsJournal of Applied Physics 122, 223102 (2017); 10.1063/1.5006934
A compact membrane-driven diamond anvil cell and cryostat system for nuclear resonant scattering at highpressure and low temperatureReview of Scientific Instruments 88, 125109 (2017); 10.1063/1.4999787
Structural, vibrational, and electronic topological transitionsof Bi1.5Sb0.5Te1.8Se1.2 under pressure
Joon-Seok Kim,1 Rinkle Juneja,2 Nilesh P. Salke,3 Witold Palosz,4
Venkataraman Swaminathan,5 Sudhir Trivedi,4 Abhishek K. Singh,2 Deji Akinwande,1
and Jung-Fu Lin3,61Department of Electrical and Computer Engineering, The University of Texas at Austin, Austin, Texas 78705,USA2Materials Research Centre, Indian Institute of Science, Bangalore 560012, India3Center for High Pressure Science and Technology Advanced Research, Shanghai 201203,People’s Republic of China4Brimrose Corporation, 19 Loveton Circle, Hunt Valley Loveton Center, Sparks, Maryland 21152, USA5U.S. Army RDECOM-ARDEC, Fuze Precision Armaments Directorate, Picatinny Arsenal, New Jersey 07806,USA6Department of Geological Sciences, The University of Texas at Austin, Austin, Texas 78712, USA
(Received 10 December 2017; accepted 4 March 2018; published online 20 March 2018)
Topological insulators have been the subject of intense research interest due to their unique surface
states that are topologically protected against scattering or defects. However, the relationship
between the crystal structure and topological insulator state remains to be clarified. Here, we show
the effects of hydrostatic pressure on the structural, vibrational, and topological properties of the
topological insulator Bi1.5Sb0.5Te1.8Se1.2 up to 45 GPa using X-ray diffraction and Raman spectros-
copy in a diamond anvil cell, together with first-principles theoretical calculations. Two pressure-
induced structural phase transitions were observed: from ambient rhombohedral R�3m phase to amonoclinic C2/m phase at �13 GPa, and to a disordered I4/mmm phase at �22 GPa. In addition, thealloy undergoes several electronic transitions within the R�3m phase: indirect to direct bulk band gaptransition at �5.8 GPa, bulk gap closing with an appearance of Dirac semimetal (DSM) state at�8.2 GPa, and to a trivial semimetal state at �12.1 GPa. Anomalies in c/a ratio and Raman fullwidth at half maximum that coincide with the DSM phase suggest the contribution of electron-
phonon coupling to the transition. Compared to binary end members Bi2Te3, Bi2Se3, and Sb2Te3, the
structural phase transition and anomaly were observed at higher pressures in Bi1.5Sb0.5Te1.8Se1.2.
These results suggest that the topological transitions are precursors to the structural phase transitions.
Published by AIP Publishing. https://doi.org/10.1063/1.5018857
Topological insulators (TIs) have attracted research
interest in the last several years, especially due to their con-
ducting edge states (in 2D TIs) or surface states (in 3D TIs)
that are topologically protected against backscattering and
cannot be passivated or destroyed by impurities or imperfec-
tions.1–4 This leads to “dissipationless” transport by the edge
or surface states that could be realized in a variety of applica-
tions including spintronics and quantum computing, and pos-
sibly create the elusive “Majorana fermion.”5 Among the
many TIs that have been identified, the metal chalcogenides
of the A2B3 (A¼Bi, Sb; B¼ S, Se, Te) series and their solidsolutions have been studied extensively from the perspective
of topological behavior as well as thermoelectric proper-
ties.6–10 Specifically, the composition of Bi1.5Sb0.5Te3-ySeywith y¼�1.2 was found to have the highest bulk resistivity,making the compound optimal for studying the surface trans-
The TI states of the A2B3 chalcogenide family are likely
closely related to their crystal structures. Reportedly, R�3mcrystals such as Bi2Te3, Sb2Te3, and Bi2Se3 are TIs, whereas
Pnma crystals such as Sb2Se3, Bi2S3, and Sb2S3 are topologi-
cally trivial in ambient conditions.11 Therefore, it is of great
importance to understand the role of crystal structure in the
topological behavior. An effective method for probing this
relationship is via the application of hydrostatic pressure,
which is a powerful means to modulate lattice parameters and
crystal structures of a material, as well as its electronic struc-
tures and topological states.12,13 Pressure-induced crystal
structural transitions in the R�3m structured chalcogenide fam-ily have been well explored, and their electronic topological
transitions (ETTs) within the TI phase are also reported.14–20
On the contrary, Pnma-structured chalcogenides remain struc-
turally stable up to 25 GPa, and their pressure-induced ETTs
are under debate.21–26 It is notable that a pressure-induced TI
state in Sb2Se3 has been reported, despite some outstanding
debates relating to the pressure transmitting medium
(PTM).22,27,28 Importantly, the relationship between crystal
phase transitions and topological transitions (e.g., whether the
surface TI state is exclusively dependent, or irrelevant to the
crystal structure) remains to be clarified.22,29,30
In this paper, we report a combined theoretical and exper-
imental investigation of the effect of hydrostatic pressure on
the topological insulator quaternary alloy Bi1.5Sb0.5Te1.8Se1.2.
Two structural phase transitions were observed from X-ray
diffraction (XRD) and Raman spectroscopy and confirmed by
0021-8979/2018/123(11)/115903/11/$30.00 Published by AIP Publishing.123, 115903-1
JOURNAL OF APPLIED PHYSICS 123, 115903 (2018)
first-principles calculations: from the ambient pressure rhom-
bohedral R�3m phase to a monoclinic C2/m phase at �13 GPa,and to a tetragonal disordered I4/mmm phase at �22 GPa.Furthermore, within the ambient R�3m phase, a series of elec-tronic transitions were demonstrated by the evolution of the
band structure as a function of pressure. The bulk indirect
band gap of the quaternary alloy undergoes indirect-to-direct
(I-to-D) band gap transition at �5.8 GPa. At �8.24 GPa, thebulk band gap closes and develops a linear crossing of bands
to form a 3D Dirac semimetal (DSM) state. On further
increase in pressure, the system becomes a normal metal
before it undergoes the first structural phase transition to the
metallic C2/m and I4/mmm phases. Concomitant with the
pressure-induced electronic transitions, various observations
from experiments also revealed profound changes at these
transitions, such as c/a ratio anomaly from XRD, and pressurecoefficient change, and full width at half maximum (FWHM)
anomalies from Raman spectroscopy. This result implies that,
although closely related, the surface states of TIs could be
modulated without change in crystal structure under hydro-
static pressures. Also, in comparison to binary end member
compounds, the Bi1.5Sb0.5Te1.8Se1.2 alloy showed structural
phase transition and other anomalies at higher pressures.
Change in axis compressibility and increase in electron-
phonon coupling (EPC) are suggested to be precursors of the
Growth of Bi1.5Sb0.5Te1.8Se1.2
Bi1.5Sb0.5Te1.8Se1.2 single crystals were grown in a two-
step process. The material was first synthesized by a modi-
fied vertical Bridgman technique similar to that reported by
Wang et al.9 Stoichiometric quantities of high purity (�5 N)metals of bismuth (5 N), antimony (5 N), selenium (6 N) and
tellurium (7 N) were vacuum sealed (10�6 Torr) in a fused
silica ampoule and melted at 900 �C for two days and slowlycooled to room temperature. The reacted material was then
resealed under vacuum in a growth ampoule with a taper.
The ampoule was heated to 900 �C for two days, cooleddown to 550 �C over 180 h, and held at that temperature for4 days before being quenched in liquid nitrogen and brought
to room temperature. The resulting crystal was highly crys-
talline and could be cleaved or exfoliated using the Scotch
High pressure Raman and X-ray diffractionexperiments
A symmetric diamond anvil cell with a pair of 350-lmdiameter diamond culets was used for the high-pressure experi-
ments. Rhenium gaskets pre-indented to �40 lm in thicknesswere drilled at the center to form the sample chamber with a
diameter of �200 lm. A piece of Bi1.5Sb0.5Te1.8Se1.2 wascleaved and then placed near the center of the sample chamber,
along with a ruby sphere used as the pressure indicator. The
shift of ruby R1 line was used to calibrate the pressure in situwith uncertainty of
based on the iterative Green’s function method48 based on
the tight-binding Hamiltonian from the maximally localized
Wannier functions (MLWF),47 as implemented in the
RESULTS AND DISCUSSION
X-ray diffraction and the structures
X-ray diffraction patterns of Bi1.5Sb0.5Te1.8Se1.2 were
taken up to 45 GPa in order to study the structural behavior of
the quaternary alloy. Figure 1 shows the selected XRD patterns,
and all XRD patterns collected up to 45 GPa are provided in
supplementary material Fig. S1. The Bi1.5Sb0.5Te1.8Se1.2 crys-
tallizes in rhombohedral structure with space group R�3m atambient pressure [Phase I; Figs. 2(a) and S2 (supplementary
material)]. With increasing pressure, the first structural phase
transition was observed in the pressure range of 13–15 GPa,
where new X-ray diffraction peaks appeared and co-existed
with Phase I. Observed above the transition was a monoclinic
phase (Phase II) with space group C2/m [Figs. 2(b) and S3
(supplementary material)]. Further increase in pressure resulted
in an additional transition to a tetragonal I4/mmm phase [Phase
III; Figs. 2(c) and S4 (supplementary material)] at 22–24 GPa,
which persisted up to the highest pressure carried out in the
present study. This structural sequence observed is similar with
parent compound Bi2Se3.16,50 Unit cell volume per formula
unit for each of the three phases is fitted using a third order
Birch-Murnaghan equation of state (EoS) in Fig. 3(a).51,52
Volume collapse of 3.52% and 2.32% was observed across
the first and second phase transitions, respectively. Bulk mod-
ulus at ambient conditions (K0), first derivative of the bulkmodulus at ambient conditions (K0
0), and zero pressure vol-ume per formula unit (V0/Z) for the three phases are given inTable I. K0 values obtained for Bi1.5Sb0.5Te1.8Se1.2 in phase
R�3m, C2/m, and I4/mmm were 52(2), 61(2), and 66(6) GPa,respectively. For phase R�3m and C2/m, K0 values are compa-rable to reported bulk moduli of parent compound Bi2Se3(48–53 GPa, and 60–64 GPa, respectively), despite the com-
position closer to Bi2Te3.16,50 In the I4/mmm phase, however,
K0 for Bi1.5Sb0.5Te1.8Se1.2 is observed to be much lower com-
pared to Bi2Se3. It is suggested that alloying with Sb2Te3 does
not alter the structure but dramatically softens the I4/mmm
phase. It is notable that a few weak peaks coexisting with
phases C2/m and I4/mmm in the pressure range of 16 to
30 GPa were observed. These peaks could presumably be
attributed to the C2/c phase, but they are too weak to draw a
Figures 3(b) and 3(c) show the normalized lattice param-
eters and axial ratio c/a as a function of pressure for the ambi-ent R�3m phase. We have also fitted pressure-dependent a andc lattice parameters using a modified Birch-Murnaghan EoS,as shown in Fig. S5 (supplementary material).16,50 The Ka,0
FIG. 1. X-ray diffraction data of Bi1.5Sb0.5Te1.8Se1.2 at selected pressures.
Phase I, II, and III correspond to R�3m, C2/m, and I4/mmm phases, respec-tively. Peaks marked with # and * indicate the emergence of C2/m and I4/
mmm phases, respectively. Major peaks from each phase are marked with
hkl indices. Inset shows the enlarged view around 7.7� at 22 GPa.
FIG. 2. The unit cells (left) and the corresponding Brillouin zones (right) of
quaternary alloy Bi1.5Sb0.5Te1.5Se1.5 in three different phases, (a) R�3m, (b)C2/m, and (c) I4/mmm. Orange arrows in the Brillouin zones represent
high-symmetry directions for band structures.
115903-3 Kim et al. J. Appl. Phys. 123, 115903 (2018)
and Kc,0 values were 56(4) and 47(2) GPa, respectively. Due
to the anisotropy of compressibility between intra-quintuple
layers (QL) and van der Waals type inter-QL, the axial cparameter is more compressible than the axial a parameter.12
However, c/a ratio showed an anomalous minimum at�7 GPa. Anomalous minimum followed by an increase inthe c/a ratio is frequently regarded as indicative of ETTor Lifshitz transition, despite existing debates on the ori-
gin.16,29,53–56 Polian et al.55 reported for Bi2Te3 that the c/aanomaly is due more to the pressure variation, or EoS
anomaly, of the in-plane lattice parameter rather than the out-
of-plane lattice parameter. In Bi1.5Sb0.5Te1.8Se1.2, the c/aanomaly was observed at a higher pressure (�7 GPa) that iscomparable to the value of �8.2 GPa at which the theoreticalcalculations predict an isostructural ETT from a topological
insulator to a three-dimensional DSM. Raman spectra as a
function of pressure, as discussed latter, also revealed signifi-
cant changes in the linewidths at �7 GPa. Based on theseobservations, it is surmised that the c/a anomaly in the quater-nary alloy is also related to an isostructural transition of topo-
To confirm the experimentally observed phase transi-
tions as a function of pressure, different phases were mod-
eled using the special quasirandom algorithm (SQS),57,58
which is a very useful modeling approach especially for the
case of disordered alloys. These SQSs mimic the relevant
local atomic structure of the random alloy, thereby providing
a complete representation of its electronic structure.57 In the
present work, the SQSs are generated for three different
phases of the quaternary alloy, namely R�3m, C2/m, and I4/mmm. The choice of the size of the supercell to generate the
periodic structure (having integer number of each element
after generating the supercell) depends on the concentration
of each element in the alloy. To handle the system computa-
tionally, the minimum possible supercell size of 2 � 2 � 2 istaken for all the three phases with the alloy concentration of
Bi1.5Sb0.5Te1.5Se1.5, instead of Bi1.5Sb0.5Te1.8Se1.2.
The primitive unit cells of the SQSs in the three phases
R�3m, C2/m, and I4/mmm and the corresponding Brillouinzones are shown in Figs. 2(a)–2(c). The total number of atoms
in the unit cell are 40, 80, and 40 for R�3m, C2/m, and I4/mmm, respectively, where in each of these phases, 25% of the
total Bi sites are replaced by Sb atoms and 50% of the Te sites
are replaced by Se atoms in the primitive unit cells of Bi2Te3using quasi-random approach. These structures are then
relaxed, and the optimized parameters are a¼ b¼ c¼ 20.7 Å;a¼ 8.4 Å, b¼ 16.9 Å, c¼ 20.1 Å; and a¼ b¼ c¼ 20.2 Å forR�3m, C2/m, and I4/mmm, respectively. Since we have used aprimitive cell for the DFT calculations, we can only compare
the bulk modulus, its pressure derivative, and the volume per
formula unit for these phases, instead of lattice parameters.
These values are summarized in Table II. The slight difference
from the experimentally reported values (Table I) may be due
to the difference in the concentration of modeled system from
the experimental one. Further, the phase transitions between
these phases are determined by calculating the energy/f.u. as a
function of the volume/f.u., as well as the enthalpy difference
relative to R�3m phase as shown in Figs. 4(a) and 4(b). Theambient pressure phase R�3m undergoes a phase transition at13.7 GPa to C2/m phase. On further increase in pressure, a
second phase transition to I4/mmm phase occurs at 24.7 GPa.
The transition pressures match closely with the experimental
To investigate the electronic and topological properties,
electronic band dispersions were calculated. The electronic
band structures for the R�3m phase with and without spin-orbit coupling (SOC) are shown in Figs. 5(a) and 5(b), and
the band structures for the two high pressure phases are
shown in Fig. S7 (supplementary material). The ambient
pressure phase is a direct band gap semiconductor without
SOC. However, due to the presence of heavy elements, the
dispersion of states both in the valence and conduction bands
are affected by the inclusion of SOC, causing the phase to
become an indirect band gap semiconductor. Interestingly,
TABLE I. Bulk modulus (K0) and first derivative of bulk modulus (K00) at
ambient conditions, and zero pressure volume per formula unit (V0/Z) for allthe three phases of Bi1.5Sb0.5Te1.8Se1.2.
Phase K0 (GPa) K00 V0/Z (Å
R�3m 52 (2) 4 152.1 (7)
C2/m 61 (2) 2.4 (2) 146.4
I4/mmm 66 (6) 4 134 (2)
FIG. 3. (a) Unit cell volume as a function of pressure, fitted using a third-
order Birch-Murnaghan equation of state. (b) Normalized a and c latticeparameters and (c) axial ratio c/a as a function of pressure for ambient rhom-bohedral R�3m phase of Bi1.5Sb0.5Te1.8Se1.2.
TABLE II. Theoretically calculated Bulk modulus (K0), and first derivative
of bulk modulus (K00) at ambient conditions, and zero pressure volume performula unit (V0/Z) for all the three phases of Bi1.5Sb0.5Te1.5Se1.5.
Phase K0 (GPa) K00 V0/Z (Å
R�3m 44.81 4.11 158.30
C2/m 53.32 3.26 149.55
I4/mmm 55.14 4.65 145.63
115903-4 Kim et al. J. Appl. Phys. 123, 115903 (2018)
the orbital contribution also changes its order across the
Fermi level around the C point when SOC is applied. In theabsence of SOC, the valence band maxima (VBM) at the Cpoint has major contributions from Te-px and Se-px orbitals,and minor contribution from Bi-s orbitals (maximum contri-bution from Bi-px orbitals), whereas the conduction bandminima (CBM) has large contribution from the Bi-px orbital,as shown in the inset of Fig. 5(a). When SOC is applied, the
valence bands around the C point acquire major contributionfrom Bi-px orbital and the conduction bands from Te-px andSe-px orbitals, as presented in the inset of Fig. 5(b). Thisindicates the inversion in the band character between the px-orbitals of the atoms in the alloy with the inclusion of SOC.
Hence, the quaternary alloy in its parent phase is a topologi-
cal insulator even after alloying Bi2Te3 with Se and Sb. The
non-trivial topology in the parent phase is further confirmed
by topological invariant Z2 through the evolution of Wannier
charge centers. The Z2 for this phase is 1, and thus has non-
To benchmark the reliability of our predictions, we fur-
ther calculated Z-terminated (001) Bloch spectral functions
with SOC for bulk as well as for both bulk and surface, based
on the idea of the bulk-edge correspondence of topological
insulators.41 The tight-binding model, based on maximally
localized Wannier functions, reproduces the DFT band struc-
ture, as shown in Fig. S6 (supplementary material) and simu-
lates the ARPES with the calculated surface density of
states. The computed ARPES in Fig. 5(d) clearly shows the
Dirac cone-like surface states, thereby confirming the non-
Having determined the ambient pressure phase to be a
topological insulator and the higher pressure phases as nor-
mal metals, we are thus interested in determining the evolu-
tion of the band structure and the electronic topology of the
FIG. 4. Calculated (a) total energy per
formula unit (f.u.) as a function of vol-
ume and (b) enthalpy difference per
formula unit relative to ambient phase
R�3m as a function of pressure for thethree phases. The total energy and
enthalpy difference is per formula unit.
The pressure corresponding to volume
is calculated using third-order Birch-
Murnaghan isothermal equation of
FIG. 5. Band structure of
Bi1.5Sb0.5Te1.5Se1.5 R�3m phase (a)before and (b) after inclusion of spin-
orbit coupling (SOC). The insets show
the inversion of the major orbital con-
tributions and the character of bands
near the C point, before and afterincluding SOC. Calculated (001)
Bloch spectral function with SOC for
(c) the bulk only and (d) both surface
and bulk. The Bloch spectral function
simulates the angle-resolved photo-
emission spectroscopy using the
Wannier function-based tight-binding
approach. The dark blue and dark red
indicate the minimum and maximum
intensity of the computed ARPES,
respectively. The cyan lines near the
Gamma point in (d) depict the surface
state contribution as a Dirac cone.
115903-5 Kim et al. J. Appl. Phys. 123, 115903 (2018)
R�3m phase before it undergoes its first phase transition.Hence, the band structures in the R�3m phase at various pres-sures are examined, and selected band structures at particular
pressures are shown in Fig. 6. As discussed previously, at
zero pressure, the quaternary alloy is a topological semicon-
ductor, with indirect bulk band gap having VBM at ZjN andCBM at MjR. With an increase in pressure, the conductionbands start to move down along ZjN direction, whereas theCBM along MjR direction starts to move up slightly. At5.80 GPa, the alloy becomes a direct band gap semiconduc-
tor, with both VBM and CBM at the ZjN high symmetrypoint. Upon further increase in the pressure, the dispersion
along the ZjN–C high symmetry direction comes closer tothe Fermi-level, whereas the remaining states are gapped
along the other high symmetry directions. At 8.24 GPa, the
band gap along the ZjN–C direction vanishes completely,creating a linear touching of bands. The ambient topological
phase of quaternary alloy thus undergoes a transition to a
non-trivial Dirac semimetal (DSM) state. Accordingly, the
surface state will mix with bulk state and lose its topologi-
cally protected state as the bulk band gap collapses.11,59 On
increasing the pressure above 8.24 GPa, the states causing
the linear dispersion start to move up above the Fermi level,
as the states along other high symmetry directions move
FIG. 6. The evolution of the band structure of Bi1.5Sb0.5Te1.5Se1.5 in the R�3m phase as a function of pressure.
115903-6 Kim et al. J. Appl. Phys. 123, 115903 (2018)
closer to the Fermi-level. At 12.09 GPa, which is below the
first phase transition pressure to the C2/m phase, the system
becomes a normal metal. The band dispersions for the high-
pressure C2/m and I4/mmm phases show topologically triv-
ial and metallic behavior (Fig. S7, supplementary material).
It is notable that since DFT has a tendency to underestimate
the band gap, and the modeled system has slightly different
concentration than the experimental one, the theoretical val-
ues of the band gap, bulk modulus as well as the transition
pressures will be slightly different from those observed
Raman spectra were measured as a function of pressure
up to 30.7 GPa, and selected spectra are shown in Fig. 7(a).
The phase transitions were observed with good agreement
with XRD and theoretical predictions. At 10.1 GPa, two new
peaks denoted as P1 and P2 appeared at 25–50 cm�1, clearly
indicating the first phase transition. Peak P3, which is rela-
tively isolated and well-defined, also showed abrupt changes
in its FWHM and intensity with the transition (Fig. S8, sup-
plementary material). At 24.1 GPa, all the features in the
Raman spectra vanished, confirming the second phase transi-
tion to the disordered I4/mmm phase. It should be noted that
Raman spectroscopy probes the material close to the surface,
in contrast to XRD, and it is therefore likely that the phonon
spectra from the surface layer are more affected at the onset
of the transition.
Listed in Table III are the observed Raman peak posi-
tions derived from Lorentzian fitting of the line shapes. The
R�3m phase has two transverse (Eg) and two longitudinal(A1g) Raman-active zone-center phonon modes, and the C2/m
phase has 15 Raman active modes (10Agþ 5Bg).16,17,19,59,60
FIG. 7. (a) Raman spectra of the quaternary Bi1.5Sb0.5Te1.8Se1.2 alloy at selected pressures. Peak positions and FWHM of peaks are obtained by Lorentzian fit-
ting of the observed Raman line shapes, as illustrated at 1.9, 10.1 and 15.6 GPa. Green and red lines represent individual Lorentzian fits and sum of the fitted
peaks, respectively. (b) Raman peak positions as a function of pressure. Vertical dashed line indicates the first appearance of phase transition. Raman shifts of
modes (c) P3 and P4, and (d) P7 and P8 as a function of pressure (GPa) are enlarged, showing changes of pressure coefficient in P3 and P4. The vertical error
bars in (c) and (d) are errors of Lorentzian fitting.
115903-7 Kim et al. J. Appl. Phys. 123, 115903 (2018)
Alloying can induce continuous shift of the Raman frequencies
with the composition (one-mode behavior), discontinuities and
peak splitting for intermediate value of composition (two-
mode behavior), or disorder-related modes.13,61,62 The E1g andA11g modes exhibit one-mode behavior upon metal or chalco-gen alloying, whereas E2g and A
21g modes exhibit two-mode
behavior upon chalcogen alloying.61,63 In this regard, the fre-
quencies and number of Raman peaks of Bi1.5Sb0.5Te1.8Se1.2are not necessarily identical to those of binary end members.
For example, P3 could be assigned as A11g mode based on theproximity of the frequency. However, it is unlikely a mode
from a specific binary compound, but likely originated from a
continuous frequency shift with respect to the compositional
alloying. On the other hand, P4-7 are results of both one-mode
and two-mode behavior. By comparing the frequencies to the
binary end members and close component BiSbTe2Se, it is
suggested that P4-5 and P6-7 have originated from E2g and A21g
modes, respectively.61,64 The large (small) pressure coefficient
of P4 (P7), which will be discussed shortly, also confirms the
origin of the Raman modes.16–19,29 P1 and P2 peaks in C2/m
phase are suggested to be A1g or B1g mode, based on the fre-
quencies and their negligible pressure dependence.16,17,19
Further theoretical and experimental work is suggested to iden-
tify the origin of the two peaks. The highest energy mode (P8)
at �225 cm�1 is likely a chalcogen A1 mode, which is a signof crystallized chalcogen defects.65–67 Note that due to the
notably weak intensity and high frequency, the influence of P8
on the analysis of P1-7 is marginal. Also, P8 does not show a
monotonic increase in its intensity (inset of Fig. S9, supple-
mentary material) despite repeated Raman measurements on
the same spot, which implies that the laser beam does not
induce ongoing damage to the sample.
Figure 7(b) shows the positions of the Raman peaks P1-
P8 as a function of pressure. Peaks P3-P7 hardened with
increasing pressure, due to the decreasing bond lengths under
pressure. The peak positions of selected peaks up to �9 GPaare enlarged in Figs. 7(c) and 7(d). P8 showed clear redshift
with a pressure coefficient of �2.88 cm�1 GPa�1 [Fig. 7(d)],in good agreement with previous reports.65–67 From linear
fits of regions below and above 4 GPa, the pressure coeffi-
cients of P3 and P4 exhibit clear decrease, whereas those of
P7 and P8 show very little change. The changes in pressure
coefficients are also observed for the A11g and E2g modes of
binary Bi2Te3,17 Bi2Se3,
16 and Sb2Te3,19 speculated to be an
indication of an isostructural ETT or Lifshitz transition.
However, our DFT calculations do not reveal any anomalous
topological behavior near �4 GPa, other than the indirect-to-direct (I-to-D) band gap transition at �5.80 GPa (Fig. 6). Beraet al. related the pressure coefficient change in Bi2Se3 to anisostructural transition featuring rapid decrease in c/a ratio andincrease in internal bond angle a.29 However, such changes ina-axis and c-axis compressibility could be related to the rapidand heterogeneous changes in band structures, such as rapid
lowering of VB, particularly at ZjN direction. Further studiesare warranted to identify the origin of the pressure coefficient
change of the Raman modes in Bi1.5Sb0.5Te1.8Se1.2. It is nota-
ble that the Ne pressure medium crystallizes at 4.8 GPa, but
non-hydrostaticity starts to develop only at higher pressures of
15–20 GPa.33,68 Also, considering the stable FWHM of P3, the
crystallization of Ne medium is unlikely to cause the pressure
coefficient change. Thermal shifting of the Raman peaks could
be also ruled out since the E2g and A21g modes in Bi2Te3 family
have similar temperature-dependent shifts.69
The FWHMs of the peaks P4-P7 from Bi1.5Sb0.5Te1.5Se1.5are shown in Fig. 8, with linear fits. The FWHMs of P4 and
P5 peaks were suppressed up to �7 GPa and increased sub-stantially in the pressure range 7–11 GPa. The FWHMs
reached maxima at �11.5 GPa, followed by rapid decreases.Considering that the increase in FWHMs is rather gradual
TABLE III. Raman modes observed in Fig. 7.
Proximity to observed modes in
P1 29 (10 GPa) A1g or B1g (C2/m)
P2 43 (10 GPa) A1g or B1g (C2/m)
P3 72 A11gP4 116 E2gP5 133 E2gP6 158 A21gP7 172 A21gP8 225 Chalcogen A1
FIG. 8. FWHM of Raman peaks (a) P4 and P5, and (b) P6 and P7 as a function of pressure (GPa). The vertical error bars are errors of Lorentzian fitting.
115903-8 Kim et al. J. Appl. Phys. 123, 115903 (2018)
compared to the abrupt changes in P1-P3 with phase transition,
and the fact that the FWHMs decrease after the maxima, the
peak broadenings are unlikely due to the emergence of the
new phase. Instead, in the sense that the linewidth of Raman
peaks is a measure of electron-phonon coupling (EPC), the
changes in FWHMs as a function of pressure imply an abrupt
increase in EPC.70,71 The anomalous FWHM jumps in P4 and
P5 in the pressure range 7–11 GPa coincide with the c/a anom-aly from XRD and the transition to a DSM state from DFT cal-
culations. It is suggested that the increase in the EPC assists
phonon-mediated renormalization of the electronic structure,
and leads to the DSM state and elimination of surface states.72
The FWHM anomalies were absent in P6 and P7, which we
have attributed to longitudinal vibrations, supporting the con-
tention that the ETT signature is related more to the in-plane
than the out-of-plane characteristics.60
Figure 9 summarizes reported structural phase transi-
tions, TI states, and reported anomalies of Bi2Te2, Bi2Se3,
Sb2Te3, Sb2Se3, and Bi1.5Sb0.5Te1.8Se1.2 (from this study) as
a function of pressure.14–20,22,27–29,50,55,73–77 The first struc-
tural phase transition of Bi1.5Sb0.5Te1.8Se1.2, from R�3m toC2/m at 13–15 GPa, is consistent with that reported in other
binary compounds such as Bi2Te3,17,73 Bi2Se3,
Sb2Te3.15,19,75 Interestingly, the structural transition is
observed at a higher pressure than the binary end members
(�7–10 GPa). The delayed structural transitions could be
attributed to the atomic disorders within the pnictogen and
chalcogen layers. Nam et al. have reported that with introduc-tion of Sb, the pnictogen layer develops a random distribution
of Bi/Sb atoms. In addition, disordered chalcogens could con-
tribute to the disordered topography, possibly up to �1% ofc-lattice constant.63 The second structural phase transition ofBi1.5Sb0.5Te1.8Se1.2 to I4/mmm phase resembles the structural
transition of Bi2Se3. Although the composition of the alloy is
closest to Bi2Te3, introduction of Se resulted in the I4/mmm
structure, instead of Im�3m structure. The C2/c phase was notas clearly observed in the Bi1.5Sb0.5Te1.8Se1.2 as in Bi2Se3.
Comparable with the delayed first structural transition, the
c/a ratio anomaly and Raman FWHM anomaly (noted in Fig.9 as “p” and “w,” respectively) of the Bi1.5Sb0.5Te1.8Se1.2 were
observed at higher pressures than those of the binary com-
pounds.16–19,26,27 The minimum in c/a ratio and FWHM anom-aly have been observed below 5 GPa in case of binary
compounds, compared to �7 GPa in Bi1.5Sb0.5Te1.8Se1.2. It isconceivable that the c/a anomalies occur when the vdW-likeinterlayer bonds are compressed enough to be as incompress-
ible as intra-layer covalent bonds, and a further increase in
pressure results in the structural phase transitions. In this sense,
the c/a anomaly could be regarded as a precursor to the struc-tural phase transition. The c/a anomaly is also closely accom-panied by the Raman FWHM anomaly, which likely promotes
the DSM state and dismantles the surface TI state. It could be
considered that the TI state is encased in the R�3m crystalphase, but only before the structural transition is imminent.
FIG. 9. Pressure-dependent phase diagram of Bi2-xSbxTe3-ySey binary compounds and Bi1.5Sb0.5Te1.8Se1.2. Values for binary compounds are adapted from
references.14–19,22,50,73–75,77 Vertical error bars indicate the variation of transition pressures from different reports. Regions dotted in red indicate TI states,
albeit the upper boundaries are not clearly defined. Reported anomalies that are attributed to have topological origin are marked as horizontal bars and charac-
ters as noted in the top right panel. Anomalies are adapted from references.16–20,27–29,55,76 Lower-right corner is a schematic showing the phase diagram of the
Bi2-xSbxTe3-ySey compounds at ambient conditions.
115903-9 Kim et al. J. Appl. Phys. 123, 115903 (2018)
We have carried out a detailed study of the effects of
hydrostatic pressure on the structural, vibrational, and topologi-
cal properties of topological insulator Bi1.5Sb0.5Te1.8Se1.2 using
diamond anvil cell experiments combined with ab initiodensity functional theory calculations. Two structural phase
transitions were observed up to �30 GPa: from the ambientrhombohedral R�3m phase to a monoclinic C2/m at �13 GPa,and to a disordered I4/mmm phase at �22 GPa. A series ofelectronic transitions were demonstrated within the R�3m struc-ture: (i) indirect-to-direct bulk band gap transition at �5.8 GPa,(ii) transition to 3D Dirac semimetal phase and vanishing of TI
state at �8.2 GPa, and (iii) transition to topologically trivialmetal at �12 GPa. The occurrence of the DSM state followingc/a ratio anomaly and FWHM anomalies of in-plane Ramanmodes suggests contribution of electron–phonon coupling to
the topological transition. By comparing with binary com-
pounds, the aforementioned anomalies are also suggested to be
precursors of the structural phase transition. Hydrostatic pres-
sure has proven to be effective in modulating crystal symmetry
and atomic bonds, and therefore capable of dramatically chang-
ing the electronic properties. This study on pressure-induced
structural and topological transitions in the Bi1.5Sb0.5Te1.8Se1.2provides deep insights toward understanding the surface state
properties and their relationship to crystal structure.
See supplementary material for the details of Le Bail
refinement of XRD patterns, calculated band dispersions of
high pressure phases, and intensity analysis of Raman
R.J. would like to thank Dr. Ravindra Shinde for the
help with surface state calculations. R.J. acknowledges the
Department of Science and Technology (DST), New Delhi,
India, for providing Fellowship under the INSPIRE
programme with registration number IF150848. R.J. and
A.K.S. would like to acknowledge support by the U.S. Army
RDECOM-Pacific under Contract FA5209-16-P-0090. J.-
S.K., J.-F.L., and D.A. would like to acknowledge support
by the U.S. Army Research Office under Contract W911NF-
13-1-0364. We also thank GSECARS of the Advanced
Photon Source for the use of the X-ray diffraction facility for
this project, Vitali Prakapenka for his assistance on the
diffraction experiments, and Richard Roberts for scientific
1M. Z. Hasan and C. L. Kane, Rev. Mod. Phys. 82, 3045 (2010).2X.-L. Qi and S.-C. Zhang, Rev. Mod. Phys. 83, 1057 (2011).3Y. Ando, J. Phys. Soc. Jpn. 82, 102001 (2013).4Y. Ando and L. Fu, Annu. Rev. Condens. Matter Phys. 6, 361 (2015).5C. Kane and J. Moore, Phys. World 24, 32 (2011).6Z. Ren, A. A. Taskin, S. Sasaki, K. Segawa, and Y. Ando, Phys. Rev. B
82, 241306(R) (2010).7Z. Ren, A. A. Taskin, S. Sasaki, K. Segawa, and Y. Ando, Phys. Rev. B
84, 165311 (2011).8T. Arakane, T. Sato, S. Souma, K. Kosaka, K. Nakayama, M. Komatsu, T.
Takahashi, Z. Ren, K. Segawa, and Y. Ando, Nat. Commun. 3, 636(2012).
9W. Wang, L. Li, W. Zou, L. He, F. Song, R. Zhang, X. Wu, and F. Zhang,
Sci. Rep. 5, 7931 (2015).10S. K. Mishra, S. Satpathy, and O. Jepsen, J. Phys.: Condens. Matter 9, 461
(1997).11H. Zhang, C.-X. Liu, X.-L. Qi, X. Dai, Z. Fang, and S.-C. Zhang, Nat.
Phys. 5, 438 (2009).12P. Lu, J.-S. Kim, J. Yang, H. Gao, J. Wu, D. Shao, B. Li, D. Zhou, J. Sun,
D. Akinwande, D. Xing, and J.-F. Lin, Phys. Rev. B 94, 224512 (2016).13J.-S. Kim, R. Ahmad, T. Pandey, A. Rai, S. Feng, J. Yang, Z. Lin, M.
Terrones, S. K. Banerjee, A. K. Singh, D. Akinwande, and J.-F. Lin, 2D
Mater. 5, 015008 (2017).14G. Xiao, K. Wang, L. Zhu, X. Tan, Y. Qiao, K. Yang, Y. Ma, B. Liu, W.
Zheng, and B. Zou, J. Phys. Chem. C 119, 3843 (2015).15Y. Ma, G. Liu, P. Zhu, H. Wang, X. Wang, Q. Cui, J. Liu, and Y. Ma,
J. Phys.: Condens. Matter 24, 475403 (2012).16R. Vilaplana, D. Santamar�ıa-P�erez, O. Gomis, F. J. Manj�on, J. Gonz�alez,
A. Segura, A. Mu~noz, P. Rodr�ıguez-Hern�andez, E. P�erez-Gonz�alez, V.Mar�ın-Borr�as, V. Mu~noz-Sanjose, C. Drasar, and V. Kucek, Phys. Rev. B84, 184110 (2011).
17R. Vilaplana, O. Gomis, F. J. Manj�on, A. Segura, E. P�erez-Gonz�alez, P.Rodr�ıguez-Hern�andez, A. Mu~noz, J. Gonz�alez, V. Mar�ın-Borr�as, V.Mu~noz-Sanjos�e, C. Drasar, and V. Kucek, Phys. Rev. B 84, 104112(2011).
18G. K. Pradhan, A. Bera, P. Kumar, D. V. S. Muthu, and A. K. Sood, Solid
State Commun. 152, 284 (2012).19O. Gomis, R. Vilaplana, F. J. Manj�on, P. Rodr�ıguez-Hern�andez, E. P�erez-
Gonz�alez, A. Mu~noz, V. Kucek, and C. Drasar, Phys. Rev. B 84, 174305(2011).
20W. Liu, X. Peng, C. Tang, L. Sun, K. Zhang, and J. Zhong, Phys. Rev. B
84, 245105 (2011).21J. Ib�a~nez, J. A. Sans, C. Popescu, J. L�opez-Vidrier, J. J. Elvira-Betanzos,
V. P. Cuenca-Gotor, O. Gomis, F. J. Manj�on, P. Rodr�ıguez-Hern�andez,and A. Mu~noz, J. Phys. Chem. C 120, 10547 (2016).
22I. Efthimiopoulos, J. Zhang, M. Kucway, C. Park, R. C. Ewing, and Y.
Wang, Sci. Rep. 3, 2665 (2013).23I. Efthimiopoulos, C. Buchan, and Y. Wang, Sci. Rep. 6, 24246 (2016).24I. Efthimiopoulos, J. Kemichick, X. Zhou, S. V. Khare, D. Ikuta, and Y.
Wang, J. Phys. Chem. A 118, 1713 (2014).25E. Zahedi and B. Xiao, Comput. Mater. Sci. 101, 301 (2015).26Y. A. Sorb, V. Rajaji, P. S. Malavi, U. Subbarao, P. Halappa, S. C. Peter,
S. Karmakar, and C. Narayana, J. Phys.: Condens. Matter 28, 015602(2016).
27A. Bera, K. Pal, D. V. Muthu, S. Sen, P. Guptasarma, U. V. Waghmare,
and A. K. Sood, Phys. Rev. Lett. 110, 107401 (2013).28W. Li, X.-Y. Wei, J.-X. Zhu, C. S. Ting, and Y. Chen, Phys. Rev. B 89,
035101 (2014).29A. Bera, K. Pal, D. V. Muthu, U. V. Waghmare, and A. K. Sood, J. Phys.:
Condens. Matter 28, 105401 (2016).30J. L. Zhang, S. J. Zhang, H. M. Weng, W. Zhang, L. X. Yang, Q. Q. Liu,
S. M. Feng, X. C. Wang, R. C. Yu, L. Z. Cao, L. Wang, W. G. Yang, H. Z.
Liu, W. Y. Zhao, S. C. Zhang, X. Dai, Z. Fang, and C. Q. Jin, Proc. Natl.
Acad. Sci. U.S.A. 108, 24 (2011).31J. C. Chervin, B. Canny, and M. Mancinelli, High Pressure Res. 21, 305
(2001).32H. K. Mao, J. Xu, and P. M. Bell, J. Geophys. Res. 91, 4673, https://
doi.org/10.1029/JB091iB05p04673 (1986).33H.-K. Mao and W. L. Mao, in Mineral Physics: Treatise on Geophysics,
edited by G. Schubert (Elsevier, Amsterdam, 2009), Vol. 2, p. 231.34W.-P. Hsieh, J. Appl. Phys. 117, 235901 (2015).35B. Le Neindre, Y. Garrabos, and R. Tufeu, Phys. A: Stat. Mech. Appl.
156, 512 (1989).36A. P. Hammersley, S. O. Svensson, M. Hanfland, A. N. Fitch, and D.
Hausermann, High Pressure Res. 14, 235 (1996).37J. Rodr�ıguez-Carvajal, in Fullprof.2k: Multi Pattern Rietveld Refinement
Program, version 1.6, July 2000.38W. Kohn and L. J. Sham, Phys. Rev. 140, A1133 (1965).39G. Kresse and J. Furthm€uller, Comput. Mater. Sci. 6, 15 (1996).40G. Kresse and J. Furthm€uller, Phys. Rev. B 54, 11169 (1996).41P. E. Bl€ochl, Phys. Rev. B 50, 17953 (1994).42G. Kresse and D. Joubert, Phys. Rev. B 59, 1758 (1999).43J. P. Perdew, K. Burke, and M. Ernzerhof, Phys. Rev. Lett. 77, 3865
(1996).44A. van de Walle, P. Tiwary, M. de Jong, D. L. Olmsted, M. Asta, A. Dick,
D. Shin, Y. Wang, L. Q. Chen, and Z. K. Liu, Calphad 42, 13 (2013).
115903-10 Kim et al. J. Appl. Phys. 123, 115903 (2018)
45A. A. Soluyanov and D. Vanderbilt, Phys. Rev. B 83, 235401 (2011).46R. Yu, X. L. Qi, A. Bernevig, Z. Fang, and X. Dai, Phys. Rev. B 84,
075119 (2011).47A. A. Mostofi, J. R. Yates, G. Pizzi, Y.-S. Lee, I. Souza, D. Vanderbilt,
and N. Marzari, Comput. Phys. Commun. 185, 2309 (2014).48M. P. L. Sancho, J. M. L. Sancho, J. M. L. Sancho, and J. Rubio, J. Phys.
F: Met. Phys. 15, 851 (1985).49Q. Wu and S. Zhang, see https://github.com/quanshengwu/wannier_tools
for WannierTools code, a tool for the investigation of novel topological
materials.50J. Zhao, H. Liu, L. Ehm, D. Dong, Z. Chen, and G. Gu, J. Phys.: Condens.
Matter 25, 125602 (2013).51F. Birch, Phys. Rev. 71, 809 (1947).52F. D. Murnaghan, Finite Deformation of an Elastic Solid (John Wiley &
Sons, Inc., New York, 1951).53A. B. Garg, V. Vijayakumar, P. Modak, D. M. Gaitonde, R. S. Rao,
B. K. Godwal, and S. K. Sikka, J. Phys.: Condens. Matter 14, 8795(2002).
54B. K. Godwal, S. Meenakshi, P. Modak, R. S. Rao, S. K. Sikka, V.
Vijayakumar, E. Bussetto, and A. Lausi, Phys. Rev. B 65, 140101(R)(2002).
55A. Polian, M. Gauthier, S. M. Souza, D. M. Trichês, J. Cardoso de Lima,
and T. A. Grandi, Phys. Rev. B 83, 113106 (2011).56A. Nakayama, M. Einaga, Y. Tanabe, S. Nakano, F. Ishikawa, and Y.
Yamada, High Pressure Res. 29, 245 (2009).57A. Zunger, S. H. Wei, L. G. Ferreira, and J. E. Bernard, Phys. Rev. Lett.
65, 353 (1990).58S. H. Wei, L. G. Ferreira, J. E. Bernard, and A. Zunger, Phys. Rev. B 42,
9622 (1990).59L. Fu, C. L. Kane, and E. J. Mele, Phys. Rev. Lett. 98, 106803 (2007).60V. Chis, I. Y. Sklyadneva, K. A. Kokh, V. A. Volodin, O. E.
Tereshchenko, and E. V. Chulkov, Phys. Rev. B 86, 174304 (2012).61W. Richter, H. Kohler, and C. R. Becker, Phys. Status Solidi B 84, 619
(1977).62J.-S. Kim, S. T. Moran, A. P. Nayak, S. Pedahzur, I. Ruiz, G. Ponce, D.
Rodriguez, J. Henny, J. Liu, J.-F. Lin, and D. Akinwande, 2D Mater. 3,025003 (2016).
63H. Nam, Y. Xu, I. Miotkowski, J. Tian, Y. P. Chen, C. Liu, M. Z. Hasan,
W. Zhu, G. A. Fiete, and C.-K. Shih, J. Phys. Chem. Solids (published
online).64N. H. Tu, Y. Tanabe, K. K. Huynh, Y. Sato, H. Oguro, S. Heguri, K.
Tsuda, M. Terauchi, K. Watanabe, and K. Tanigaki, Appl. Phys. Lett. 105,063104 (2014).
65R. Vilaplana, O. Gomis, F. J. Manj�on, H. M. Ortiz, E. P�erez-Gonz�alez, J.L�opez-Solano, P. Rodr�ıguez-Hern�andez, A. Mu~noz, D. Errandonea, V. V.Ursaki, and I. M. Tiginyanu, J. Phys. Chem. C 117, 15773 (2013).
66V. P. Cuenca-Gotor, J. A. Sans, J. Ib�a~nez, C. Popescu, O. Gomis, R.Vilaplana, F. J. Manj�on, A. Leonardo, E. Sagasta, A. Su�arez-Alcubilla, I. G.Gurtubay, M. Mollar, and A. Bergara, J. Phys. Chem. C 120, 19340 (2016).
67G. P. Lindberg, R. E. Tallman, R. Lauck, M. Cardona, X. Liu, J. K.
Furdyna, and B. A. Weinstein, Phys. Status Solidi B 250, 711 (2013).68S. Klotz, J. C. Chervin, P. Munsch, and G. Le Marchand, J. Phys. D: Appl.
Phys. 42, 075413 (2009).69B. Irfan, S. Sahoo, A. P. S. Gaur, M. Ahmadi, M. J. F. Guinel, R. S.
Katiyar, and R. Chatterjee, J. Appl. Phys. 115, 173506 (2014).70A. Sharafeev, V. Gnezdilov, R. Sankar, F. C. Chou, and P. Lemmens,
Phys. Rev. B 95, 235148 (2017).71X. Zhu, L. Santos, C. Howard, R. Sankar, F. C. Chou, C. Chamon, and M.
El-Batanouny, Phys. Rev. Lett. 108, 185501 (2012).72O. Delaire, K. Marty, M. B. Stone, P. R. C. Kent, M. S. Lucas, D. L.
Abernathy, D. Mandrus, and B. C. Sales, Proc. Natl. Acad. Sci. U.S.A.
108, 4725 (2011).73L. Zhu, H. Wang, Y. Wang, J. Lv, Y. Ma, Q. Cui, Y. Ma, and G. Zou,
Phys. Rev. Lett. 106, 145501 (2011).74Z. Yu, L. Wang, Q. Hu, J. Zhao, S. Yan, K. Yang, S. Sinogeikin, G. Gu,
and H.-k. Mao, Sci. Rep. 5, 15939 (2015).75J. Zhao, H. Liu, L. Ehm, Z. Chen, S. Sinogeikin, Y. Zhao, and G. Gu,
Inorg. Chem. 50, 11291 (2011).76P. P. Kong, F. Sun, L. Y. Xing, J. Zhu, S. J. Zhang, W. M. Li, Q. Q. Liu,
X. C. Wang, S. M. Feng, X. H. Yu, J. L. Zhu, R. C. Yu, W. G. Yang, G. Y.
Shen, Y. S. Zhao, R. Ahuja, H. K. Mao, and C. Q. Jin, Sci. Rep. 4, 6679(2014).
77G. Liu, L. Zhu, Y. Ma, C. Lin, J. Liu, and Y. Ma, J. Phys. Chem. C 117,10045 (2013).
115903-11 Kim et al. J. Appl. Phys. 123, 115903 (2018)